- Nano Express
- Open Access
Effect of a Rubidium Chloride Carrier Confinement Layer on the Characteristics of CsPbBr3 Perovskite Light-Emitting Diodes
Nanoscale Research Letters volume 17, Article number: 2 (2022)
This work describes the effect of a rubidium chloride (RbCl) interlayer in CsPbBr3 perovskite light-emitting diode (LED) structures. RbCl crystallites exhibited polyhedral structures and lattice parameters similar to those of CsPbBr3 perovskite crystallites. The lattice mismatch between the RbCl interlayer and CsPbBr3 active layer was only approximately 2%. The devices exhibited the best quality and performance when RbCl was used as the nucleation and carrier confinement layer. The crystallite sizes of CsPbBr3 with 0.2-, 0.5-, and 1-nm-thick RbCl bottom layers were 55.1, 65.4, and 55.1 nm, respectively. The full width at half maximum (FWHM) of the photoluminescence (PL) emission peak for CsPbBr3 with the RbCl bottom layer was 0.096 eV.
Halide perovskite materials have been extensively studied and are often applied in different photocatalytic and photovoltaic devices owing to their high absorption coefficient and low-cost processing [1,2,3,4,5,6]. Perovskite is a light-emitting diode (LED) material that shows potential for use as a display light source in future because of its impressive properties, including high color purity, high photoluminescence quantum yield, and low nonradiative recombination ratio [7,8,9]. A common engineering method used to boost the luminance of perovskite LEDs is to modify the interfaces between the cathode, electron transport layer, perovskite active layer, hole transport layer, and anode, thereby maximizes carrier injection to the fullest extent possible, except for optimizing the perovskite grain size and conductivity of the layers.
Rubidium chloride (RbCl) has been used as an electron transport layer (ETL) with organic light-emitting diodes (OLEDs) to increase electroluminescent efficiency by lowering the effective electron-injecting barrier height and enhancing the electron–hole pair recombination rate [10,11,12]. Alkali metal cations have also been used to prevent phase segregation of perovskite materials and dopants in PEDOT:PSS used in perovskite solar cell structures, thereby modifying the interface between PEDOT:PSS and the perovskite active layer [13,14,15]. In addition, RbCl has been employed with the solution method to dope CsPbBr3 perovskite films used for blue LEDs . However, interface engineering is important for optoelectronic device structures. Therefore, in this work, we investigate the effect of the RbCl layer used as an ETL in CsPbBr3 perovskite light-emitting diodes to improve carrier injection and the buffer layer between PEDOT:PSS and CsPbBr3 perovskite active layers to increase the power conversion efficiency.
Materials and Syntheses
CsPbBr3 perovskite LEDs were fabricated on indium tin oxide (ITO)-coated glass substrates (Ruilong Ltd., Taiwan). Cesium bromide (CsBr, 99.99%), lead iodide (PbI2, 98%), dimethyl sulfoxide (DMSO, 99.9%), rubidium chloride (RbCl, 99.8%), polyethylene oxide (PEO, Mv 400,000), and 1,3,5-benzinetriyl)-tris(1-phenyl-1-H-benzimidazole (TPBi, 99%) were obtained from UniRegion Bio-Tech Ltd. (Taiwan).
First, a CsPbBr3 perovskite solution was prepared: 96 mg of cesium bromide (CsBr) and 110 mg of lead bromide (PbBr2) were dissolved in 1 mL of dimethyl sulfoxide (DMSO) and then stirred and degassed at 70 °C overnight to produce solution A. Then, 10 mg of polyethylene oxide (PEO) was dissolved in 1 mL of DMSO and stirred and degassed at 70 °C overnight to produce solution B. Then, 0.5 mL of solution A and 20 mg of TPBi powder were added to solution B and stirred until it became completely transparent.
ITO glass substrates were cleaned with acetone, alcohol, and isopropanol by ultrasonic cleaning for 15 min. PEDOT:PSS was spin-coated on the ITO substrate at 5000 rpm for 60 s and then baked at 140 °C for 15 min. For structure 2, the CsPbBr3 perovskite solution was spin-coated on the PEDOT:PSS layer at 3000 rpm for 60 s and baked at 80 °C for 10 min. The RbCl upper layer was deposited on the CsPbBr3 perovskite layer by the thermal evaporation method. Subsequently, 13-nm-thick TPBi and 100-nm-thick Ag were sequentially deposited by thermal evaporation on the RbCl upper layer. The whole LED structure and process flow are shown in Fig. 1a. For structure 3, the RbCl layer was deposited on the PEDOT:PSS layer by the thermal evaporation method. The CsPbBr3 perovskite solution was spin-coated on the RbCl bottom layer at 3000 rpm for 60 s and baked at 80 °C for 10 min. Subsequently, 13-nm-thick TPBi and 100-nm-thick Ag were sequentially deposited on the CsPbBr3 perovskite by thermal evaporation. The whole LED structure and process flow are shown in Fig. 1b. In this work, three thicknesses (0.2, 0.5, and 1 nm) were employed for the RbCl layer.
The morphologies of CsPbBr3 films with and without the RbCl layer were observed using field-emission scanning electron microscopy (FESEM, ZEISS Sigma, ZEISS, Munich, Germany). Crystallite sizes and lattice parameters were estimated using X-ray diffraction (X’Pert PRO MRD, PANalytical, Almelo, Netherlands). Optical characteristics were measured by a fluorescence spectrophotometer (F-7000, Hitachi, Tokyo, Japan). The optoelectronic properties of LEDs were measured using a Keithley 2420 source meter and PR-670 spectroradiometer (JADAK, New York, USA). All characterizations were measured at room temperature.
Results and Discussion
Three structures were studied in this work, as shown in Fig. 2a. Figure 2b–h show top-view FESEM images of the three structures. Figure 2b shows the morphology of structure 1, which is a control sample without the RbCl layer, for comparison with other structures. Figure 2c–e are top views of structure 2 with various thicknesses of the RbCl upper layer. The particle sizes on the surface are larger than those of the control sample without the RbCl layer. Figure 2f–h are top views of structure 3 with various thicknesses of the RbCl bottom layer. The insets of FESEM images in Fig. 2b–h are particle size distribution histograms. The average particle sizes were 120, 180–230, and 80–120 nm for structures 1, 2, and 3, respectively. The particle on the surface were smaller and denser than those of the control sample without the RbCl layer. This may be because the RbCl bottom layer assists nucleation of the CsPbBr3 perovskite film.
Figure 3 presents the XRD patterns for various structures and thicknesses of the RbCl layers. For the structure without a RbCl layer, six clear diffraction peaks at 15.28°, 21.43°, 30.42°, 35.28°, 37.63°, and 50.73° were observed. They correspond to the (110), (112), (220), (210), (211), and (044) planes of orthorhombic CsPbBr3 crystallites, respectively [17,18,19]. For the structure with a RbCl layer, one diffraction shoulder at 30.72° was observed that corresponds to the RbCl dopant due to diffusion effect [20, 21]. The ionic Rb+ and Cs+ have similar ionic radii and the Rb+ substitution could stabilize the orthorhombic CsPbBr3 phase, as a resulting of diffraction peak of orthorhombic RbPbBr3 [20, 22]. To compare CsPbBr3 film quality, crystallite sizes were estimated by Scherrer's equation [23, 24]. The crystallite sizes of CsPbBr3 without and with 0.2-, 0.5-, and 1-nm-thick RbCl bottom layers were 53.5, 55.1, 65.4, and 55.1 nm, respectively. Therefore, the RbCl bottom layer improved the CsPbBr3 crystallites due to their similar polyhedral structures.
Figure 4 shows absorbance spectra for CsPbBr3 films with and without RbCl layers. The absorption edges of all samples appeared at 520 nm in the absorbance spectra. The optical band gap of the samples was calculated to be approximately 2.385 eV. This result is consistent with the band gap of the CsPbBr3 film. The band gap of the RbCl layer is approximately 4.8 eV. Thus, it was transparent to visible light. Additionally, a noticeable absorption band was seen at 425 nm and is attributed to absorption by the trans-isomers of 4-(nitrophenyl)azo groups in the PEDOT:PSS layer [25, 26].
Photoluminescence (PL) emission spectra of the CsPbBr3 films with and without the RbCl layer are shown in Fig. 5a. The emission peaks in the PL spectra of all samples are at 518 nm. This peak corresponds to a band gap of 2.394 eV [27, 28]. Clearly, the intensities for CsPbBr3 films with the RbCl bottom layer are higher than those for CsPbBr3 film alone and CsPbBr3 films with the RbCl upper layer. The PL intensity responds to the carrier lifetime caused by defect-induced recombination. The FWHM of the emission peak of CsPbBr3 with the RbCl bottom layer is 0.096 eV. It is less than 0.1 eV for CsPbBr3 with the RbCl upper layer and 0.126 eV for CsPbBr3 without the RbCl layer owing to the better crystallite quality. The charge carrier recombination kinetics of CsPbBr3 films with and without a RbCl layer were investigated by time-resolved photoluminescence (TRPL) measurements, as shown in Fig. 5b. Table 1 lists the parameters obtained from fits of the TRPL spectra. The RbCl bottom layer obviously improved the carrier lifetime, and the carrier lifetime was increased slightly by the RbCl upper layer. In other words, RbCl positioned as the bottom layer of the CsPbBr3 film had a better impact than the upper layer on the quality of CsPbBr3 films.
Figure 6a and b are plots of the energy levels of structure 2 and structure 3. In structure 2, the RbCl layer was formed as an electron transport layer on the CsPbBr3 active layer. In structure 3, the RbCl layer was inserted as a carrier confinement layer under the CsPbBr3 active layer to improve the efficiency of electron–hole recombination and enhance the performance of CsPbBr3 perovskite LEDs . Figure 6c–f plot the electroluminescence (EL), current density, luminescence, and external quantum efficiency of CsPbBr3 perovskite LEDs with and without a RbCl layer. Remarkably, the performance of CsPbBr3 LEDs with RbCl bottom layers was superior to that of CsPbBr3 LEDs without and with a RbCl upper layer owing to improvement in crystallite quality for the CsPbBr3 active layer and carrier confinement effect of the RbCl bottom layer, although the turn-on voltage increased from 5 to 5.5 V due to insertion of the RbCl layer, as shown in Fig. 6d. Another factor of performance improvement may be contributed to that Rb+ dopant reduces the surface defects and non-radiative recombination of CsPbBr3 active layer due to passivation, and then increases the carrier lifetime, as shown in Fig. 5b [16, 20, 21]. As shown in Fig. 6c, the emission peaks for all devices appeared at approximately 514 nm and were consistent with the peaks in the PL spectra, as shown in Fig. 5. The inset of Fig. 6c shows a photograph of an operating LED. The intensities of the EL spectra for CsPbBr3 LEDs with RbCl bottom layers were higher than those of CsPbBr3 LEDs without and with a RbCl upper layer. The best luminescence and external quantum efficiency were 9718 cd/m2 at a bias of 8.5 V and 1.29% at a bias of 7.5 V, respectively. These values constituted improvements of 33% and 262%, respectively. In addition, in this work, CsPbBr3 LEDs with RbCl upper layers did not show the effects of an electron transport layer, similar to an OLED structure, according to Fig. 6c–f. It means that the RbCl impossibly behaves as an electron transport layer in perovskite LEDs.
In summary, the effect of rubidium chloride (RbCl) interlayers in CsPbBr3 perovskite structures of light-emitting diodes (LED) was studied. When using RbCl as the nucleation layer, the CsPbBr3 perovskite exhibited the best quality and performance. The crystallite sizes of CsPbBr3 with 0.2-, 0.5-, and 1-nm-thick RbCl bottom layers were 55.1, 65.4, and 55.1 nm, respectively. The performance of CsPbBr3 LEDs with RbCl bottom layers was superior to those of CsPbBr3 LEDs without and with RbCl upper layers. The best luminescence and external quantum efficiencies were 9718 cd/m2 at a bias of 8.5 V and 1.29% at a bias of 7.5 V, respectively. These values constituted improvements of 33% and 262%, respectively. This may be due to several factors: the crystallite quality of the improved CsPbBr3 active layer, stabile CsPbBr3 crystalline, surface passivation strategy of the CsPbBr3 active layer, and the carrier confinement effect of the RbCl layer.
Availability of Data and Materials
All the data are fully available without restrictions.
- CsPbBr3 :
Cesium lead tri-bromide
- PbBr2 :
Field-emission scanning electron microscopy
Indium tin oxide
Poly (3,4-ethylenedioxythiophene) polystyrene sulfonate
Organic light-emitting diode
Schanze KS, Kamat PV, Yang P, Bisquert J (2020) Progress in perovskite photocatalysis. ACS Energy Lett 5:2602–2604
Teh YW, Chee MK, Kong XY, Yong S-T, Chai S-P (2020) An insight into perovskite-based photocatalysts for artificial photosynthesis. Sustain Energy Fuels 4:973–984
Kojima A, Teshima K, Shirai Y, Miyasaka T (2009) Organometal halide perovskites as visible-light sensitizers for photovoltaic cells. J Am Chem Soc 131(17):6050–6051
National Renewable Energy Laboratory (2021) Best research-cell efficiencies. Available online: https://www.nrel.gov/pv/assets/pdfs/best-research-cell-efficiencies.20200104.pdf. Accessed 4 Jan 2021
Liu Z, Krückemeier L, Krogmeier B, Klingebiel B, Márquez J, Levcenko S, Öz S, Mathur S, Rau U, Unold T, Kirchartz T (2019) Open-circuit voltages exceeding 1.26 V in planar methylammonium lead iodide perovskite solar cells. ACS Energy Lett 4(1):110–117
Gao B, Meng J, Lu J, Zhao R (2020) CH3NH3PbI3 perovskite solar cells with efficiency over 22% fabricated by green antisolvent method. Mater Lett 274:127995
Zhang Q, Tavakoli MM, Gu L, Zhang D, Tang L, Gao Y, Guo J, Lin Y, Leung S-F, Poddar S (2019) Efficient metal halide perovskite light-emitting diodes with significantly improved light extraction on nanophotonic substrates. Nat Photon 10:727
Park J, Jang HM, Kim S, Jo SH, Lee TW (2020) Electroluminescence of perovskite nanocrystals with ligand engineering. Trends Chem 2:837–849
He Q, Mei E, Liang X, Xiang W (2021) Ultrastable PVB films-protected CsPbBr 3/Cs4PbBr6 perovskites with high color purity for nearing Rec. 2020 standard. Chem Eng J 419:129529
Lü Z, Deng Z, Du H, Li D, Zou Y, Xu D, Chen Z, Wang Y (2009) The effect of rubidium chloride on properties of organic light-emitting diodes. Solid State Electron 53:1154–1158
Lü Z, Wang Y, Zou Y, Du H, Chen Z, Deng Z (2010) The effect of alkaline metal chlorides on the properties of organic light-emitting diodes. J Lumin 130:387–391
Lü Z, Deng Z, Hou Y, Xu H (2012) Similarities and differences of alkali metal chlorides applied in organic light-emitting diodes. Thin Solid Films 525:106–109
Zhang S, Tang M-C, Fan Y, Li R, Nguyen NV, Zhao K, Anthopoulos TD, Hacker CA (2020) Role of alkali-metal cations in electronic structure and halide segregation of hybrid perovskites. ACS Appl Mater Interfaces 12:34402–34412
Liu X, Li B, Zhang N, Yu Z, Sun K, Tang B, Shi D, Yao H, Ouyang J, Gong H (2018) Multifunctional RbCl dopants for efficient inverted planar perovskite solar cell with ultra-high fill factor, negligible hysteresis and improved stability. Nano Energy 53:567–578
Wang H, Xu Y, Wu J, Chen L, Yang Q, Zhang B, Xie Z (2020) Bright and color-stable blue-light-emitting diodes based on three-dimensional perovskite polycrystalline films via morphology and interface engineering. J Phys Chem Lett 11:1411–1418
Wang HL, Zhao XF, Zhang BH, Xie ZY (2019) Blue perovskite light-emitting diodes based on RbX-doped polycrystalline CsPbBr3 perovskite films. J Mater Chem C 7:5596–5603
Zhang L, Yuan F, Dong H, Jiao B, Zhang W, Hou X, Wang S, Gong Q, Wu Z (2018) One-step co-evaporation of all-inorganic perovskite thin films with room-temperature ultralow amplified spontaneous emission threshold and air stability. ACS Appl Mater Interfaces 10:40661–40671
Tenailleau C, Aharon S, Cohen B-E, Etgar L (2019) Cell refinement of CsPbBr3 perovskite nanoparticles and thin films. Nanoscale Adv 1:147–153
Zhang M, Zheng Z, Fu Q, Chen Z, He J, Zhang S, Yan L, Hu Y, Luo W (2017) Growth and characterization of all-inorganic lead halide perovskite semiconductor CsPbBr3 single crystals. Cryst Eng Commun 19:6797–6803
Todorović P, Ma DX, Chen B, Quintero-Bermudez R, Saidaminov MI, Dong YT, Lu ZH, Sargent EH (2019) Spectrally tunable and stable electroluminescence enabled by rubidium doping of CsPbBr3 nanocrystals. Adv Opt Mater 7:1901440
Geng YX, Yang BB, Xiang YR, Shi MM, Hu RR, Guo CF, Li YF, Zou J (2021) Preparation and research of perovakite quantum dots power based on RbCl doped CsPbBr3. Chem Sel 6:8422–8425
Xiao JW, Liang Y, Zhang SY, Zhao YZ, Li YJ, Chen Q (2019) Stabilizing RbPbBr3 perovskite nanocrystals through Cs+ substitution. Chem Eur J 25:2597–2603
West AR (2014) Solid state chemistry and its applications. Wiley, Hoboken
Chen L-C, Tseng Z-L, Chen C-C, Chang SH, Ho C-H (2016) Fabrication and characteristics of CH3NH3PbI3 perovskite solar cells with molybdenum-selenide hole-transport layer. Appl Phys Exp 9:122301
Kalachyova Y, Guselnikova O, Postnikov P, Fitl P, Lapcak L, Svorcik V, Lyutakov O (2018) Reversible switching of PEDOT:PSS conductivity in the dielectric–conductive range through the redistribution of light-governing polymers. RSC Adv 8:11198–11206
Yeung CL, Charlesworth S, Iqbal P, Bowen J, Preece JA, Mendes PM (2013) Different formation kinetics and photoisomerization behavior of self-assembled monolayers of thiols and dithiolanes bearing azobenzene moieties. Phys Chem Chem Phys 15:11014–11024
Gan Z, Zheng F, Mao W, Zhou C, Chen W, Bach U, Tapping P, Kee TW, Davis JA, Jia B (2019) The optical properties of Cs4PbBr6–CsPbBr3 perovskite composites. Nanoscale 11:14676–14683
Sun C, Wei J, Zhao J, Jiang Y, Wang Y, Hu H, Wang X, Zhang Y, Yuan M (2021) Hard and soft Lewis-base behavior for efficient and stable CsPbBr3 perovskite light-emitting diodes. Nanophotonics 10:2157–2166
Jiang J, Sun X, Chen XC, Wang BW, Chen ZZ, Hu Y, Gio YW, Zhang LF, Ma Y, Gao L, Zhanf FS, Jin L, Chen M, Ma ZW, Zhou YY, Padture NP, Beach K, Terrones H, Shi YF, Gall D, Lu TM, Wertz E, Feng J, Shi J (2019) Carrier lifetime enhancement in halide perovskite via remote epitaxy. Nat Commun 10:4145
This work was supported by the Ministry of Science and Technology (Taiwan) under contract No. 110-2221-E-027-125.
This work was supported by the Ministry of Science and Technology (Taiwan) under contract No. 110-2221-E-027-125.
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
About this article
Cite this article
Li, CT., Lee, KL., Wang, SF. et al. Effect of a Rubidium Chloride Carrier Confinement Layer on the Characteristics of CsPbBr3 Perovskite Light-Emitting Diodes. Nanoscale Res Lett 17, 2 (2022). https://doi.org/10.1186/s11671-021-03641-9
- RbCl carrier confinement layer
- Light-emitting diodes